Rheological approach to select most suitable associative thickener for water-based polymer dispersions and paints
- 248 Downloads
In the 1980s, a new class of thickeners, i.e., associative thickener (AT), was introduced for water-based coatings to improve their rheology. Principally, they work by associating with polymer particles present in the paint. Manufacturers of ATs provide some generic guidelines to choose them based on economy, regulatory restrictions, and polymer type; however, it is very difficult to choose suitable ATs until and unless their interactions with polymer particles are studied by rheology. This article focuses on developing a rheological approach to identify a suitable AT for a paint formulation. In this approach, a rheology viscosity curve was used on AT–emulsion polymer mix and AT–emulsion polymer–surfactant mix to short-list a suitable AT. Subsequently, the shortlisted ATs were tested in the paint formulation to study their efficacy. Commonly used, hazardous air pollutants (HAPs)-free, commercially available ATs, viz. hydrophobically modified ethoxylated urethane thickener (HEUR) and hydrophobically modified poly(acetal- or ketal-polyether) thickener (HMPE), were selected to study their interaction with a unique surfactant-stabilized acrylic–polyurethane hybrid emulsion. A range of acrylic–polyurethane hybrid emulsions were prepared by increasing the polyurethane content in the emulsion. As the polyurethane content increased in the emulsion polymer, the thickening efficiency of AT decreased.
KeywordsAcrylic–polyurethane hybrid emulsion polymer Associative thickeners Water-based paints Rheology
Authors are thankful to Asian paints management for giving permission to submit this paper for international publication. Authors are also thankful to Mr. Girish Gurjar, Mr. Vijay Shigwan, and Mr. Sushant Barve from Modern Instrumentation Laboratory for their help in FTIR, PSA, and DSC. Thanks are also due to Dr. Subrahmanya Shreepathi, Dr. Sisirkumar Mandal, Dr. Subarna Shyamroy, Dr. Raja Krishnamurthy, and Dr. Venkata Chada for their suggestion and encouragement.
- 1.Eley, RR, “Applied Rheology in the Protective and Decorative Coating Industry.” Rheol. Rev., 173–240 (2005)Google Scholar
- 2.Shay, GD, “Ch-30, Thickeners and Rheology Modifiers.” In: Koleske, JV (ed.), Paints and Coating Testing Manual, 14th Ed. Gardner-Sward Handbook (ASTM Manual Series) 268 London (1995)Google Scholar
- 8.Hegedus, CR, Kloiber, KA, “Aqueous Acrylic-Polyurethane Hybrid Dispersions and Their Use in Industrial Coatings.” J. Coat. Technol., 68 (860) 39–48 (1996)Google Scholar
- 19.Doolan, JG, Cody, CA, “A Pourable Water Dispersible Thickening Composition for AQUEOUS System.” US patent CA2144101C, 1995Google Scholar
- 20.Kruse, U, Tituscille, Crowley, BC, River, T, both of N. J., Wilbur S. Mardis, East Amherst, N. Y. “Water Dispersible Modified Polyurethane Thickener with Improved High Shear Viscosity in Aqueous System.” US Patent 5023309, 1991Google Scholar
- 21.Sau, AC, “Hydrophobically Modified Poly(Acetal-Polyethers).” US patent 5574127, 1996Google Scholar
- 22.Hendel, RA, Yan, L, Cheng, L, “Methods for Controlling Silica Scale in Aqueous Systems.” US Patent 7316787 B2, 2008Google Scholar
- 23.Sau, AC, “Supression of Aqueous Viscosity of Associative Polyacetal–Polyethers.” US Patent 6809132 B2, 2004Google Scholar
- 24.Patton, TC, Paint Flow and Pigment Dispersion, 2nd ed. Interscience Publishers, New York (1964)Google Scholar
- 25.Auschra, C, Romero, IG, Willerich, I, Reichardt, R, Muenzenberg, C, Martinez, E, He, H, “The Role of Thickeners in Optimizing Coating Formulations.” In: ChinaCoat 2014, 19th China Exhibition for Coatings, Printing Inks and Adhesives, Guanzhou, China, Dec. 2014, Paper no-7Google Scholar